November 21, 1997

Contract \# **TW-0928**

SPECIAL SPECIFICATION

SECTION 09900-S

[PAINTING]{.underline}

Page

[PART 1 - GENERAL]{.underline}

1.01 Description of Work 2

1.02 References 4

1.03 Submittals 4

1.04 Quality Assurance 5

1.05 Delivery, Storage and Handling 6

1.06 Job Conditions 6

PART 2 - PRODUCTS

2.01 Manufacturers 7

2.02 Masonry Block Filler 7

2.03 Primers/Sealers 7

2.04 Exterior Finish Paint Material 7

2.05 Interior Finish Paint Material 8

PART 3 - EXECUTION

3.01 Examination 8

3.02 Preparation 8

3.03 Application 10

3.04 Cleaning 12

3.05 Protection 12

3.06 Exterior Paint Schedule 13

3.07 Interior Paint Schedule 14

3.08 Fire Protection Painting 16

SPECIAL SPECIFICATION

SECTION 09900-S

[PAINTING]{.underline}

# PART 1 - GENERAL

## 1.01 [DESCRIPTION OF WORK]{.underline}

A. [Scope]{.underline}: This section includes surface preparation,
painting, and finishing of exposed interior and exterior items and
surfaces, including touch-up painting on prefinished items. Surface
preparation, priming, and finish coats specified in this section are in
addition to shop-priming and surface treatment specified under other
sections.

B. [Definition]{.underline}: The term \"paint\" as used herein includes
emulsions, primers, enamels, stains, varnishes, sealers, cement-emulsion
filler, and other coatings, whether used as prime, intermediate, or
finish coat.

C. [Surfaces To Be Painted]{.underline}

1\. Paint all exposed surfaces whether or not colors are designated in
articles 3.06 and 3.07, except where surface or material is specifically
indicated not to be painted or to remain natural.

2\. Where an item or surface is not specifically mentioned, paint the
same as similar adjacent materials or surfaces.

3\. If color or finish is not designated, the Sandia Delegated
Representative (SDR) will select from standard colors or finishes
available.

4\. Surfaces listed in articles 3.06, 3.07 and 3.08, other than those
listed in subarticles 1.01 D and E, will receive the surface
preparation, paints, and number of coats prescribed in the schedule.

5\. Electrical items to be painted include, but are not limited to:

a\. Exposed conduit and fittings, (except in E below)

b\. Exposed cabinets, enclosures, junction boxes, and pull boxes

c\. Exposed hangers

D. [Surfaces Not Requiring Painting]{.underline}

1\. Prefinished items including the following factory-finished
components:

a\. Metal toilet enclosures, unless otherwise specified

b\. Acoustic materials

c\. Architectural woodwork and casework

d\. Finished mechanical and electrical equipment

e\. Switchgear

f\. Distribution cabinets

2\. Concealed surfaces including wall or ceiling surfaces in unfinished
spaces.

a\. Foundation spaces

b\. Duct shafts

c\. Elevator shafts

3\. Factory finished surfaces such as:

a\. Anodized aluminum

b\. Stainless steel

c\. Chromium plate

d\. Glass

e\. Bronze and brass

4\. Operating parts including moving parts of operating equipment such
as the following:

a\. Valve and damper operators

b\. Linkages

c\. Sensing devices

d\. Motor and fan shafts

E. [Surfaces For Which Painting Is Prohibited]{.underline}

1\. Sprinkler heads.

2\. Fire and smoke detectors.

3\. Conduit and equipment in equipment rooms, unless otherwise
specified.

4\. Equipment in hazardous (classified) locations.

5\. [Labels]{.underline}: Do not paint over Underwriter\'s Laboratories,
Factory Mutual or other code-required labels or equipment name,
identification, performance rating, or nomenclature plates.

6\. Concealed auto-releasing sprinkler head covers (i.e.; escutcheon
plates).

7\. Glass, brass, or chrome plated portions of fire protection system
control valves (PIVs, gate valves, etc.) hydrants and fire department
connections. (Reference NFPA 13 and Standard Specification Division 15,
Section \"Automatic Sprinkler System.\")

F. [Related Sections]{.underline}: The following sections contain
requirements that relate to this section:

1\. Division 5, Section \"Structural Steel\" for shop-priming structural
steel.

2\. Division 8, Section \"Wood Doors\" for shop-priming wood doors and
steel frames.

3\. Division 8, Section \"Steel Doors and Frames\" for shop-priming
steel doors and frames.

4\. Division 15, Section \"Automatic Sprinkler Systems\" for painting
water based fire protection systems.

## 1.02 [REFERENCES]{.underline}

A. [National Fire Protection Association (NFPA)]{.underline}

13 Standard for the Installation of Sprinkler Systems

B. [Code of Federal Regulations (CFR)]{.underline}

Title 29 Part 1910 Labor - Occupational Safety and Health Standards

Title 29 Part 1926 Safety and Health Regulations for Construction

## 1.03 [SUBMITTALS]{.underline}

The following shall be submitted in accordance with Division 1, Section
1300-S, \"Descriptive Submittals\":

A. [Product Data]{.underline}: Manufacturer\'s catalog data, label
analysis, and application instructions for each material proposed for
use.

1\. List each material and cross-reference the specific coating and
finish system and application. Identify each material by the
manufacturer\'s catalog number and general classification.

2\. Samples for initial color selection shall be in the form of
manufacturer\'s color charts.

B. [Asbestos Free and Lead Paint Free Certification]{.underline}: Submit
manufacturer\'s written certification that all materials are free of
asbestos and lead paint.

C. [Samples]{.underline}: For each color specified, apply a complete
liquid glaze coating system to representative samples of the actual
substrate to be used in the work and submit for approval. The approved
sample panels will be used for quality control in applying the glaze
coating system.

1\. Provide a list of material and application for each coat of each
sample. Label each sample as to location and application.

2\. Submit samples on the following substrates for the SDR\'s review of
color and texture only:

a\. [Concrete]{.underline}: Provide two 4 inch x 4 inch (102 mm x 102
mm) samples for each color and finish.

b\. [Gypsum Board]{.underline}: Provide one 6 inch x 6 inch (152 mm x
152 mm) sample of each color and finish.

d

c\. [Ferrous Metal]{.underline}: Provide two 4 inch x 4 inch (102 mm x
102 mm) samples of flat metal and two 8 inch (203 mm) long samples of
solid metal for each color and finish.

## 1.04 [QUALITY ASSURANCE]{.underline}

A. [Single-Source Responsibility]{.underline}: Provide primers and
undercoat paint produced by the same manufacturer of the finish coats.

B. [Coordination of Work]{.underline}: Review other sections in which
primers are provided to ensure compatibility of the total coating
systems for various substrates. On request, furnish information on
characteristics of finish materials to ensure use of compatible primers.

Notify the SDR of problems anticipated using the materials specified.

C. [Material Quality]{.underline}: Provide the manufacturer\'s best
quality trade sale paint material of the various coating types
specified. Paint material containers not displaying manufacturer\'s
product identification are not acceptable.

Proprietary names used to designate colors or materials are not intended
to imply that products named are required, or to exclude equal products
of other manufacturers.

## 1.05 [DELIVERY, STORAGE, AND HANDLING]{.underline}

A. [Deliver materials]{.underline} to the job site in the
manufacturer\'s original, unopened packages and containers bearing
manufacturer\'s name, label, and the following information:

1\. Product name or title of material

2\. Product description (generic classification or binder type)

3\. Manufacturer\'s stock number and date of manufacture

4\. Contents by volume, for pigment and vehicle constituents

5\. Thinning instructions

6\. Application instructions

7\. Color name and number

8\. VOC content

B. [Store materials]{.underline} not in use in tightly covered
containers in a well-ventilated area at a minimum ambient temperature of
45°F (7°C). Store all flammable materials not in use in Underwriter\'s
Laboratories, Inc., NFPA or other approved flammable storage cabinet.
Reference OSHA 29 CFR 1926 if storage of combustible or flammable
liquids exceed 25 gallons (94.6 liters). Maintain containers and
cabinets used for storage in a clean condition, free of foreign
materials and residue.

Protect from freezing. Keep storage area neat and orderly. Remove oily
rags and waste daily. Take necessary measures to ensure that workers and
work areas are protected from fire and health hazards resulting from
handling, mixing, and application.

## 1.06 [JOB CONDITIONS]{.underline}

A. [Apply water-based paints]{.underline} only when the temperature of
surfaces to be painted and surrounding air temperatures are between 50°F
(10°C) and 90°F (32°C).

B. [Apply solvent-thinned paints]{.underline} only when the temperature
of surfaces to be painted and surrounding air temperatures are between
45°F (7°C) and 95°F (35°C).

C. [Do not apply paint]{.underline} in snow, rain, fog, or mist, when
the relative humidity exceeds 85 percent, at temperatures less than 5°F
(3°C) above the dew point, or to damp or wet surfaces.

Painting may continue during inclement weather if surfaces and areas to
be painted are enclosed and heated within temperature and humidity
limits specified by the manufacturer during application and drying
periods.

# PART 2 - PRODUCTS

## 2.01 [MANUFACTURERS]{.underline}

[Available Manufacturers]{.underline}: Subject to compliance with
requirements, manufacturers offering products that may be incorporated
in the work include, but are not limited to, the following:

Benjamin Moore and Co. (BM)

Sherwin-Williams Company (S-W)

Wellborn Paint Manufacturing Company (W)

## 2.02 [MASONRY BLOCK FILLER]{.underline}

A. [High-Performance Latex Block Filler]{.underline}: Heavy-duty latex
block fillers used for filling open, textured interior and exterior
concrete masonry block before application of top coats.

B. [Block filler]{.underline} used under high-performance polyamide
epoxy coatings.

## 2.03 [PRIMERS/SEALERS]{.underline}

A. [Interior Latex Enamel]{.underline}: To be used as under-coat for
smooth cementitious surfaces and bare wood.

B. [Interior Latex-Based White Primer]{.underline}: Latex-based primer
coating be used on interior gypsum drywall under a flat latex paint or a
semi-gloss latex enamel.

C. [Exterior Primer Coating]{.underline}: Exterior alkyd wood primer
used for priming wood under alkyd enamels.

D. [Rust-Inhibiting Primer]{.underline}: Quick-drying, rust-inhibiting
primer used for priming ferrous metal on the exterior under high-gloss
enamel and on the interior under enamel.

E. [Galvanized Metal Primer]{.underline}: Primer used to prime interior
and exterior zinc-coated (galvanized) metal surfaces.

F. [Pigmented Sealer]{.underline}: Pigmented sealers over concrete used
under high performance polyamide epoxy coatings.

## 2.04 [EXTERIOR FINISH PAINT MATERIAL]{.underline}

A. [Exterior Acrylic]{.underline}: Quick-drying, flat, acrylic paint
used on the exterior over concrete, stucco, and masonry (including
concrete masonry block).

B. [Alkyd Enamel]{.underline}: Weather-resistant, air-drying, semi-gloss
enamel used on the exterior over prime-coated wood, and over primed
ferrous metal surfaces.

## 2.05 [INTERIOR FINISH PAINT MATERIAL]{.underline}

A. [Interior Semi-Gloss Latex Enamel]{.underline}: Semi-gloss, latex
enamel used over a primer on concrete, masonry (including concrete
masonry block), wood and hardboard, ferrous and zinc-coated (galvanized)
metal surfaces, and over a primer on gypsum drywall.

B. [Latex-Based, Interior Flat Paint]{.underline}: Ready-mixed,
latex-based paint used as a \"size\" on cotton or canvas covering over
insulation.

C. [High-Performance Polyamide Epoxy Coating]{.underline}: High-gloss
coating used over concrete and concrete masonry.

## 

## 

## PART 3 - EXECUTION

## 3.01 [EXAMINATION]{.underline}

[Examine substrates and conditions]{.underline} under which painting
will be performed for compliance with requirements for application of
paint. Do not begin paint application until unsatisfactory conditions
have been corrected. Start of painting will be construed as
Applicator\'s acceptance of surfaces and conditions within a particular
area.

## 3.02 [PREPARATION]{.underline}

A. [General Procedures]{.underline}: Remove hardware and hardware
accessories, plates, machined surfaces, lighting fixtures, and similar
items in places that are not to be painted, or provide surface-applied
protection prior to surface preparation and painting. Remove these items
if necessary for complete painting of the items and adjacent surfaces.
Clean surfaces before applying paint or surface treatments. Remove oil
and grease prior to cleaning. Schedule cleaning and painting so that
dust and other contaminants from the cleaning process will not fall on
wet, newly-painted surfaces. Following completion of painting operations
in each space or area, items shall be reinstalled in the same manner
that they were removed.

B. [Surface Preparation]{.underline}: Clean and prepare surfaces to be
painted in accordance with the manufacturer\'s instructions for each
particular substrate condition and as specified.

Provide barrier coats over incompatible primers or remove and reprime.
Notify SDR in writing when problems are anticipated in using the
specified finish-coat material with substrates primed by others.

C. [Cementitious Materials]{.underline}: Prepare concrete, concrete
masonry block, and stucco to be painted. Remove efflorescence, chalk,
dust, dirt, grease, oils, and release agents. Roughen as required to
remove glaze. If hardeners or sealers have been used to improve curing,
use mechanical methods of surface preparation.

1\. Use abrasive blast-cleaning methods if recommended by the paint
manufacturer.

2\. Determine alkalinity and moisture content of surfaces by performing
appropriate tests. Pay special attention to concrete masonry unit mortar
joints and patched concrete surfaces. If surfaces are sufficiently
alkaline to cause blistering and burning of finish paint, correct this
condition before application. Do not paint surfaces where moisture
content of surface to be painted exceeds that permitted in
manufacturer\'s printed directions.

3\. Clean concrete floors to be painted with a 5 percent solution of
muriatic acid or other etching cleaner. Flush the floor with clean water
to remove acid, neutralize with ammonia, and rinse; allow to dry and
vacuum before painting.

D. [Wood Materials]{.underline}: Clean surfaces of dirt, oil, and other
foreign substances with scrapers, mineral spirits, and sandpaper. Sand
smooth surfaces exposed to view and dust off.

1\. Scrape and clean small, dry, seasoned knots and apply a thin coat of
white shellac or other recommended knot sealer before application of
primer.

2\. Prime, stain, or seal wood to be painted immediately upon delivery.
Prime edges, ends, faces, undersides, and backsides of wood, including
cabinets, counters, cases, and paneling. After priming, fill holes and
imperfections in finish surfaces with putty or plastic wood filler. Sand
smooth when dried.

3\. When transparent finish is required, backprime with spar varnish.

4\. Seal tops, bottoms, and cutouts of unprimed wood doors with a heavy
coat of varnish or sealer immediately upon delivery to jobsite.

E. [Ferrous Metals]{.underline}: Clean nongalvanized ferrous-metal
surfaces that have not been shop-coated; remove oil, grease, dirt, loose
mill scale, and other foreign substances. Use solvent or mechanical
cleaning methods that comply with recommendations of the Steel
Structures Painting Council.

1\. Treat bare and sand-blasted or pickled clean metal with a metal
treatment wash coat before priming.

2\. Touch up bare areas and shop-applied prime coats that have been
damaged. Wire-brush, clean with solvents recommended by the paint
manufacturer, and touch up with the same primer as the shop coat.

F. [Galvanized Surfaces]{.underline}: Clean galvanized surfaces with
non-petroleum-based solvents so that the surface is free of oil and
surface contaminants. Remove pretreatment from galvanized sheet metal
fabricated from coil stock by mechanical methods.

G. [Gypsum Board]{.underline}: Surfaces shall be dry and shall have all
loose dirt and dust removed by brushing with a soft brush, rubbing with
a dry cloth, or vacuum-cleaning prior to application of first-coat
material. Repair blemishes, irregularities and damaged surfaces.

H. [Material Preparation]{.underline}: Carefully mix and prepare paint
materials in accordance with the manufacturer\'s directions.

1\. Maintain containers used in mixing and application of paint in a
clean condition, free of foreign materials and residue.

2\. Stir material before application to produce a mixture of uniform
density; stir as required during application. Do not stir surface film
into material. Remove film and, if necessary, strain material before
using.

3\. Use only thinners approved by the paint manufacturer, and only
within recommended limits. Use odorless thinner with alkyd enamel.

## 3.03 [APPLICATION]{.underline}

A. [General]{.underline}

1\. Apply paint in accordance with manufacturer\'s directions. Use
applicators and techniques best suited for substrate and type of
material being applied. Spray applications will require prior approval
from the SDR.

2\. Do not paint over dirt, rust, scale, grease, moisture, scuffed
surfaces, or conditions detrimental to formation of a durable paint
film.

3\. Surface treatments and finishes shall be as indicated in articles
3.06, 3.07 and 3.08 or as selected by SDR.

4\. Provide finish coats that are compatible with primers used.

5\. The number of coats and film thickness required is the same
regardless of the application method. Do not apply succeeding coats
until the previous coat has cured as recommended by the manufacturer.
Sand between applications where sanding is required to produce an even,
smooth surface in accordance with the manufacturer\'s directions.

6\. Apply additional coats when undercoats, stains, or other conditions
show through final coat of paint until paint film is of uniform finish,
color, and appearance. Give special attention to ensure that surfaces,
including edges, corners, crevices, welds and exposed fasteners receive
a dry film thickness equivalent to that of flat surfaces.

7\. The term \"exposed surfaces\" includes areas visible when permanent
or built-in fixtures, convector covers, covers for finned tube
radiation, grilles, and similar components are in place. Extend coatings
in these areas as required to maintain the system integrity and provide
desired protection.

8\. Paint surfaces behind movable equipment and furniture same as
similar exposed surfaces. Paint surfaces behind permanently fixed
equipment or furniture with prime coat only before final installation of
equipment.

9\. Paint interior surfaces of ducts, where visible through registers or
grilles, with a flat, nonspecular black paint.

10\. Paint back sides of access panels and removable or hinged covers to
match exposed surfaces.

11\. Finish exterior doors on tops, bottoms, and side edges same as
exterior faces.

12\. Sand lightly between each succeeding enamel or varnish coat.

13\. Omit primer on metal surfaces that have been shop-primed and touch
up painted.

B. [Scheduling Painting]{.underline}: Apply first coat to surfaces that
have been cleaned, pretreated, or otherwise prepared for painting as
soon as practicable after preparation and before subsequent surface
deterioration.

Allow time between successive coats to permit proper drying per
manufacturer\'s recommendations.

C. [Minimum Coating Thickness]{.underline}: Apply materials at not less
than the manufacturer\'s recommended spreading rate. Provide a total dry
film thickness of the entire system as recommended by the manufacturer
or as specified, whichever is greater.

D. [Mixing and Thinning]{.underline}: Unless otherwise recommended by
the manufacturer, paints may be thinned immediately prior to application
with an approved manufacturer\'s thinner and used only within
recommended limits when necessary to suit conditions of surface
temperature, weather and application methods. The use of thinner shall
not relieve the Contractor from obtaining complete hiding, full film
thickness, or required gloss. Paints of different manufacturers shall
not be mixed.

E. [Mechanical Work]{.underline}: Color-coding of mechanical piping
systems is limited to those items exposed in mechanical equipment rooms.
Paint shall be applied directly to the insulation and/or pipe on systems
which are not insulated. Label pipe systems appropriately after
painting. Painting of other mechanical items is limited to those exposed
in mechanical equipment rooms and occupied spaces except as otherwise
indicated. Use paint and color specified or other manufacturer\'s
equivalent.

> Items to be painted and color-coded include the following:

1\. [Chilled Water Systems]{.underline}: Piping, pumps, chillers, air
separators and expansion tank. Wellborn #Q13-64U, Dark Blue.

2\. [Tower Water System]{.underline}: Piping and pumps. Wellborn
#Q13-12T, Light Blue.

3\. [Steam and Condensate]{.underline}: Piping, flash tank, condensate
pump. Wellborn #Q6-23T, Yellow.

4\. [Heating Hot Water System]{.underline}: Piping, pumps, air
separator, heat exchanger and expansion tank. Wellborn #Q3-66U, Orange.

5\. [Compressed Air System]{.underline}: Piping and receiver tank.
Wellborn #Q14-57T, Gray.

6\. [Fire Protection System]{.underline}: Piping, valves, alarms and
drains. \"Fire Protection Red\" (refer to article 3.08 A and B).

7\. [Natural Gas]{.underline}: Wellborn #Q6-23T, Yellow.

8\. [Domestic Cold Water]{.underline}: Wellborn #Q10-66U, Dark Green.

9\. [Domestic Hot Water]{.underline}: Piping, pumps and heat exchanger.
Wellborn #Q9-21P, Light Green.

10\. [Non-Potable Water]{.underline}: Wellborn #Q3-66U, Orange.

F. [Prime Coats]{.underline}: Before application of finish coats, apply
a prime coat of material as recommended by the manufacturer to material
that is required to be painted or finished and has not been prime coated
by others. Recoat primed and sealed surfaces where evidence of suction
spots or unsealed areas in first coat appears, to assure a finish coat
with no burn-through or other defects due to insufficient sealing.

G. [Pigmented (Opaque) Finishes]{.underline}: Completely cover to
provide an opaque, smooth surface of uniform finish, color, appearance,
and coverage. Cloudiness, spotting, holidays, laps, brush marks, runs,
sags, ropiness, or other surface imperfections are not acceptable.

H. [Transparent (Clear) Finishes]{.underline}: Use multiple coats to
produce a glass-smooth surface film of even luster. Provide a finish
free of laps, cloudiness, color irregularity, runs, brush marks, orange
peel, nail holes, or other surface imperfections.

Provide satin finish for final coats.

I. [Completed Work]{.underline}: Match approved samples for color,
texture, and coverage. Remove, refinish, or repaint work not in
compliance with specified requirements.

## 3.04 [CLEANING]{.underline}

A. [Cleanup]{.underline}: At the end of each work day, completely remove
empty cans, rags, tools, rubbish, and other discarded paint materials
from the project site.

B. [Do not clean]{.underline} tools, brushes, applicators, etc. at the
project site unless specifically authorized by the SDR. Do not use sinks
in restrooms, janitors\' closets, or in locations where food is
prepared.

C. [Upon completion of painting]{.underline}, clean glass and
paint-spattered surfaces. Remove spattered paint by washing and
scraping, using care not to scratch or damage adjacent finished
surfaces.

## 3.05 [PROTECTION]{.underline}

A. [Protect work]{.underline} of other trades, whether to be painted or
not, against damage by painting. Correct damage by cleaning, repairing
or replacing, and repainting, as acceptable to the SDR.

B. [Provide \"wet paint\" signs]{.underline} to protect newly painted
finishes. Remove temporary protective wrappings provided by others for
protection of their work after completion of painting operations.

At completion of construction activities of other trades, touch up and
restore damaged or defaced painted surfaces.

## 3.06 [EXTERIOR PAINT SCHEDULE]{.underline}

Provide the following paint systems for the various substrates
indicated.

No primer or block filler is required on previously painted surfaces,
unless specified on Contract documents or where alkaline, moisture or
freeze-thaw cycles have caused blistering or peeling.

A. [Ferrous Metal]{.underline}: Primer is not required on shop-primed
items.

1\. [Alkyd Enamel]{.underline}: Two (2) finish coats over primer.

Primer: Rust-Inhibiting Primer

First Coat: Alkyd Enamel

Second Coat: Alkyd Enamel

2\. [Pipe and Railings Color]{.underline}: Benjamin Moore 1393

B. [Galvanized Metal]{.underline}

[Alkyd Enamel]{.underline}: Two (2) finish coats over primer.

Primer: Galvanized Metal Primer

First Coat: Alkyd Enamel

Second Coat: Alkyd Enamel

## 3.07 [INTERIOR PAINT SCHEDULE]{.underline}

[General]{.underline}: Provide the following paint systems for the
various substrates, as indicated.

No primer or block filler is required on previously painted surfaces.

A. [Concrete]{.underline} (other than concrete masonry units):

1\. [Semi-Gloss Enamel Finish]{.underline}: Three (3) coats with total
dry film thickness per manufacturer\'s recommendations.

Primer: Interior Latex Enamel

Undercoat: Interior Semi-Gloss Latex Enamel

Finish Coat: Interior Semi-Gloss Latex Enamel

2\. Polyamide Epoxy Coating: Two (2) coats of polyamide epoxy coating
over pigmented sealer.

Sealer Coat: Manufacturer\'s recommended pigmented sealer

Intermediate Coat: Polyamide Epoxy

Finish Coat: Polyamide Epoxy

3.  Basement Concrete Walls, Columns and Ceilings

Primer: 1 coat Kem Cati-Coat Epoxy Filler/Sealer @ 10 mils DFT

Finish: 2 coats Water-Based Catalyzed Epoxy 3 mils DFT/coat B70 Series

Color: White

4.  Concrete Columns in Service Galley.

Primer: 1 coat ProMar 200 Latex Wall Primer @ 1.1 mils DFT B28 Series.

Finish: 2 coats ProMar 200 Interior Latex Semi-Gloss Enamel @ 1.3 mils.

Color: White

C. [Gypsum Drywall Systems]{.underline}

1\. [Semi-Gloss Latex Enamel Finish]{.underline}: Three (3) coats with
total dry film thickness per manufacturer\'s recommendations.

Primer: Interior Latex-Based White Primer

Intermediate Coat: Interior Semi-Gloss Latex Enamel

Finish Coat: Interior Semi-Gloss Latex Enamel

Color: See Finish Key and Specifications of Materials dwg. 105632/A1 and
special finish plans dwg. Series 105632.

2\. [Basement Drywall]{.underline}

Primer: ProMar 200 Latex Wall Primer B28 Series 1.1 mils DFT

Finish: 2 coats Water-Based Catalyzed Epoxy 3 mils DFT/coat B70 Series

3.  [Service Galley]{.underline}

Primer: 1 coat Promar 200 Latex Wall Primer @ 1/1 mils DFT B28 series

Finish: 2 coats ProMar 200 Interior Latex Semi-Gloss Enamel @ 1.3 Mils
DFT. Series: B31.

D. [Woodwork and Hardboard]{.underline}

[Semi-Gloss Enamel Finish]{.underline}: Three (3) coats.

Primer: Interior Latex Enamel

Intermediate Coat: Interior Semi-Gloss Latex Enamel

Finish Coat: Interior Semi-Gloss Latex Enamel

F. [Ferrous Metal]{.underline}

1\. [Semi-Gloss Enamel Finish]{.underline}: Two (2) coats over primer
with total dry film thickness per manufacturer\'s recommendations.

Primer: Rust-Inhibiting Primer

Intermediate Coat: Interior Semi-Gloss Latex Enamel

Finish Coat: Interior Semi-Gloss Latex Enamel

2.  [Hollow Metal Doors and Frames]{.underline}

Primer: Shop primed touch-up with same primer as specified in Section
08110.

Finish: 2 coats ProMar 200 Interior Latex Gloss Enamel @ 1.5 mil DFT
B21W 200 Series

H. [Zinc-Coated Metal]{.underline}

[Semi-Gloss Finish]{.underline}: Two (2) coats over primer, with total
dry film thickness not less than 2.5 mils (0.064 mm).

Primer: Galvanized Metal Primer

Intermediate Coat: Interior Semi-Gloss Latex Enamel

Finish Coat: Interior Semi-Gloss Latex Enamel

I. [Basement Exit]{.underline} [and Service Galley and
LN~2~]{.underline} [Fill Station]{.underline} [Aisle Floor
Striping]{.underline}

Finish: 1 coat Promar Alkyd Traffic Marking Paint spread per
manufacturer's instructions.

3.08 [FIRE PROTECTION PAINTING]{.underline}

Contractor shall paint those portions of fire protection as required by
Sandia National Laboratories (SNL) as follows, except as required in
Section 1.01, E.1-5:

A. [Color Coding of Outdoor Water-Based Fire Protection
System]{.underline}

1\. [Hydrants]{.underline}: All fire hydrants shall be painted \"Traffic
Yellow.\" The top portion (bonnet) shall be reflective (glass beaded)
paint.

2\. [Post Indicator Valves]{.underline}: Sprinkler controlled post
indicator valves shall be painted \"Fire Protection Red.\" Water
distribution system division post indicator valves shall be painted
\"Traffic Yellow.\"

3\. [Water Motor Alarms]{.underline}: All water motor alarms, gongs and
sprinkler system drains through walls shall be painted \"Fire Protection
Red.\"

4\. [Sprinkler Piping]{.underline}: All sprinkler piping which is
exposed to exterior surface corrosion shall be painted \"Fire Protection
Red.\" Reference OSHA 29 CFR 1910 159(C).6.

B. [Color Coding of Indoor Water-Based Fire Protection
Systems]{.underline}

1\. [Sprinkler System]{.underline}: All sprinkler risers, including
backflow preventers, alarm check valves, dry pipe valves, pre-action and
deluge valves and accessory trim devices and piping shall be painted
\"Fire Protection Red.\"

a\. Riser pipes shall be painted up to the suspended ceiling or in areas
without ceilings, up to the first horizontal sprinkler feed main.

b\. Valve drops (e.g. inspector tests, drain lines) shall be painted
\"Fire Protection Red\" from the ceiling, or in areas without ceilings,
from the branch line downward, including fittings and pipes located
outdoors.

c\. Where other horizontal or vertical pipes are color coded, horizontal
or vertical sprinkler piping shall be painted \"Fire Protection Red.\"

d\. In no instance shall any part of a sprinkler head be painted.
Sprinkler heads which have been painted or coated except by the
manufacturer shall be replaced and shall not be cleaned by use of
chemicals, abrasives, or other means. Each sprinkler head shall be
protected with a biodegradable paper bag, that shall be removed
immediately after painting has been finished.

2\. [Sprinkler Piping]{.underline}: All sprinkler piping subject to
damage by operations (e.g. forklift, crane, robotics, chemicals) shall
be painted \"Fire Protection Red.\" Note: The paint utilized for piping
exposed to chemicals shall be a type which will resist the effects of
the chemical environment present.

C. [Labeling of Outdoor Water-Based Fire Protection System]{.underline}

1\. [Post indicator valves]{.underline} controlling sprinkler systems
shall be labeled with the building and sprinkler system riser number
which it controls.

2\. [Fire department (Siamese) connections]{.underline} shall be labeled
with the building(s), sprinkler riser(s) and number that they supply.
They shall also be labeled with the type of system (e.g. hose stations,
stand pipes or sprinklers) they supply.

3\. [Labeling shall be accomplished]{.underline} with the use of
\"Brady\" or approved equal, self-sticking labels. The color and size
shall contrast the surface which it is applied to. The labels shall be
provided and applied by SNL Fire Protection Systems Maintenance
Organization.

D. [Labeling of Indoor Water-Based Fire Protection System]{.underline}

1\. [Sprinkler System]{.underline} (e.g., inspectors tests, drain
valves) shall be labeled with all information required by NFPA Standard
No. 13.

2\. [Labeling shall be accomplished]{.underline} with the use of
permanently marked weatherproof metal or rigid plastic identification
signs. The signs shall be secured with corrosion-resistant wire, chain,
or other approved means. These signs shall be provided by the
manufacturer, manufacturer\'s representative, or installer of the
sprinkler system.

3\. [Sprinkler riser shall be labeled]{.underline} with building and
sprinkler system riser numbers. Labeling shall be accomplished with the
use of \"Brady\" or approved equal self-sticking labels. The color and
size shall contrast the surface which it is applied to. The labels shall
be provided and applied by SNL Fire Protection Systems Maintenance
Organization.

END OF SECTION